Concrete Mix Design for M35 Grade: Comparison of Indian Standard Codes, IS 10262: 2009 & IS 456:2000 with American Code, ACI 211.


 Myles Clark
 8 days ago
 Views:
Transcription
1 Concrete Mix Design for M35 Grade: Comparison of Indian Standard Codes, IS 10262: 2009 & IS 456:2000 with American Code, ACI Dada S. Patil Assistant Professor, Civil Engineering Department, AnjumanIIslam s Kalsekar Technical Campus, School of Engineering & Technology, Panvel, Navi Mumbai, Maharashtra, India *** Abstract  A rational & logical Concrete Mix Design to cater to the practical requirements plays a key role in concrete engineering. It is well established fact that the concrete is highly consumed material throughout the world. With the exponentially high demand of infrastructure facilities, the concrete requirement is on a very huge scale. Therefore, using the optimum quantities of concrete making constituent materials is of utmost importance in order to achieve the desired fresh & hardened properties. Owing to an enormous utilization of concrete in day today construction work, economy is a vital factor to be considered. In India, mix design is carried out by following the rules prescribed in IS 10262: 2009 & IS 456:2000. As a well known fact, every country has its own codes to design a concrete mix. In this paper, an attempt has been made to compare the Concrete Mix Design of M35 grade by the American Code; ACI with Indian codes IS 10262: 2009 & IS 456:2000. The outcomes are critically reviewed & the comments are given. Keywords: OPC, (w/c) ratio, nominal maximum size of aggregate, workability, slump, target mean strength, etc. 2. MIX DESIGN BY USING IS 10262: 2009 & IS 456: Stipulations for Proportioning Grade designation: M 35 Type of cement: Ordinary Portland Cement (OPC), conforming to IS: Maximum nominal size of aggregate: Exposure condition considered: Moderate (for Reinforced Concrete) For moderate exposure condition (from Table 5 of IS 456: 2000) i) Minimum cement content: ii) Maximum watercement ratio: Desired workability: Type of aggregate: Crushed angular aggregate Maximum cement content: 450 kg/m 3 IS 456: 2000) (Clause of 1. INTRODUCTION Every country has a peculiar method of carrying out the Concrete Mix Design by following the various clauses, tables & figures given in the codes of that particular country. It is obvious that these codes give important guidelines for designing a concrete mix depending upon the basic properties of constituent materials, behaviour of individual constituent, economy & many other considerations. The guidelines are proposed in such a way that the concrete is workable enough for a particular type of field application when it is in a fresh state; moreover, it caters to the need of desirable strength & durability properties, when hardened. This paper critically compares the Concrete Mix Design of M35 grade carried out by using Indian Standard codes & American code. The vital observations are presented. Conclusions are drawn based on these observations. 2.2 Test Data for Materials Specific gravity of cement: 3.15 Chemical admixture: NA Specific gravity of i) Coarse aggregate: 2.72 ii) Fine aggregate: 2.68 Sieve Analysis (coarse aggregates; 20 mm & 10 mm): Conforming to grading requirements of table 4 of IS 383:1970. Sieve analysis (Fine aggregates): Conforming to grading Zone I of table 4 of IS 383: , IRJET Impact Factor value: ISO 9001:2008 Certified Journal Page 2580
2 2.3 Target Strength for Mix Proportioning f ck = f ck + (1.65 S) Where: = Target average compressive strength at 28 days. = Characteristic compressive strength at 28 days = Standard deviation. From Table 1 of IS : 2009, Standard deviation =, For M35 concrete Therefore, target strength = = 2.4 Selection of Water  Cement Ratio & Water Content From Table 5 of IS 456:2000, maximum watercement ratio = 0.50 Adopt watercement ratio as 0.45, since the target strength is N/mm 2. From Table 2 of IS10262:2009, maximum water content = for aggregates. As per clause 4.2 of IS 10262:2009, for every increase of slump of 25 mm, the water content has to be increased by 3%. So, estimated water content for slump = ( ) = Consider it as 192 kg/m Calculation of Cement Watercement ratio = 0.45; Cement content = (192/0.45) = kg/m kg/m 3 (max. OPC permitted) > kg/m 3 > 300 kg/m 3 (min. cement content). Its complying the requirements. 2.6 Proportion of Volume of Coarse Aggregate & Fine Aggregate Content From Table 3 of IS 10262: 2009, the volume of coarse aggregates corresponding to size aggregates & fine aggregates of Zone I for (w/c) ratio of 0.50 is (w/c) ratio adopted is Therefore, Volume of coarse aggregate is required to be increased to decrease the fine aggregate content. As the watercement ratio is lower by 0.05, the proportion of volume of coarse aggregate is to be increased by 0.01 (at the rate of / for every ± 0.05 change in watercement ratio). Therefore, corrected proportion of volume of coarse aggregate for the watercement ratio of 0.45 = ( ) = Volume of fine aggregate content = = Mix Calculations The mix calculations per unit volume of concrete shall be as follows: Volume of concrete (a) =. Volume of cement (b) = (mass of cement/ specific gravity of cement) X (1/1000) = ( / 3.15) X (1/1000) = m 3. Volume of water (c) = (mass of water/ specific gravity of water) X (1/1000) = (192/1) X (1/1000) = m 3. Volume of all in aggregate (d) = a (b +c) = 1 ( ) = m 3. Mass of coarse aggregate = (d) X volume of CA X specific gravity of CA X = (0.673 X 0.61 X 2.72 X 1000) = kg. Mass of fine aggregate = (d) X volume of FA X specific gravity of FA X = (0.673 X 0.39 X 2.68 X 1000) = kg. Yield of concrete = ( ) = kg/m , IRJET Impact Factor value: ISO 9001:2008 Certified Journal Page 2581
3 2.8 Mix Proportions (kg/m 3 ), at SSD (Saturated Surface Dry) condition of Fine Aggregate & Coarse Aggregate Table 3: Approximate Mixing Water & Air Content Requirements for Different Slumps & Nominal Max. Size of Aggregates (SI Units) Table 1: Mix Proportions Cement Water FA CA (w/c) ratio MIX DESIGN BY USING ACI Let us carry out Mix Design by using ACI code. Let all the material properties be same as that in IS code Let dry rodded density of CA be 1640 kg/m Selection of WaterCement Ratio Table 4: Relationship Between (w/c) Ratio & Compressive Strength of Concrete (SI Units) American code uses the concept of dry rodded density of CA. 3.1 Choice of Slump Table 2: Recommended Slumps for various Types of Construction (SI Units) For target strength of N/mm 2, (w/c) ratio for nonair entrained concrete is 0.54, by interpolation. This is more than the maximum (w/c) ratio of 0.50 for the moderate exposure condition, as given by the Indian Code. If the (w/c) ratio given by ACI method exceeds the maximum limit of 0.50 prescribed by the Indian Standard Code (moderate exposure), the value should be discarded & (w/c) ratio of 0.50 is to be used for further calculations. Though ACI method is used for the Mix Design, the Desired slump is 75 mm (25 mm to 75 mm category from table 2). 3.2 Choice of Maximum Size of Aggregate From table 3, select Max. Aggregate Size = 19 mm, as it is closer to 20 mm size. 3.3 Estimation of Mixing Water & Air Content From table 3, W=205 litres (i. e. kg) for 19 mm aggregates & entrapped air = 2%. concreting is to be done in India & therefore, the exposure conditions must be considered from the Indian Code from durability point of view. However, if the (w/c) ratio obtained by ACI method is less than the max. limit given by IS code table, it is obvious that the value obtained is to be adopted for further calculations. 3.5 Calculation of Cement Content Mass of cement, M C = Water/ {w/c ratio} = (205/0.50) = 410 kg/m , IRJET Impact Factor value: ISO 9001:2008 Certified Journal Page 2582
4 Here, the (w/c) ratio is marginally more than that in IS It is well established fact that, as the (w/c) ratio increases, the strength shows decline in its value. However, the cement quantity is less than that in IS After trial, if the required target strength is achieved & concrete is workable for a given application, it is acceptable. Volume of cement, V c = 410/(3.15X1000)=0.130 m Estimation of CA & FA Contents 3.7 Mix Proportions (kg/m 3 ), at SSD (Saturated Surface Dry) condition of Fine Aggregate & Coarse Aggregate Table 6: Mix Proportions Cement Water FA CA (w/c) ratio Table 5: Volume of CA Per Unit Volume of Concrete (SI Units) 4. COMPARISON OF IS METHOD & ACI METHOD FOR CONCRETE MIX DESIGN Table 7: Materials Required kg/m 3 ) Met hod Cement Water FA CA (w/c) Ratio IS Let us assume that the fineness modulus of FA is 3. The sand confirms to zone I as per IS code. From table 5, for 19 mm nominal max. size of aggregate, volume of dry rodded ACI CA per unit volume of concrete is So, mass of CA, M ca = (0.6 x dry rodded density of CA) = (0.6 X 1640) = 984 kg/m 3 So, volume of CA, V ca = (M ca /Sp. gravity X 1000) = 984 / [2.72 x 1000] = m 3. Volume of FA, V fa = 1 (V c + V w + V ca + V ea) Here, V c = cement volume, V w = volume of water, V ca= volume of CA & V ea = volume of entrapped air (2%). V fa = 1  ( ) = Mass of FA, M fa = (0.284 x 1000 x 2.68) = kg. Yield of concrete = ( ) = kg/m Observations The cement content obtained by IS method is kg/m 3 ; whereas, it is 410 kg/m 3 as per ACI With the same constituent materials, water per m 3, calculated by ACI method is 13 kg (or litres) more than that obtained by IS Fine Aggregate quantity/m 3 obtained by ACI method is kg more than that obtained by IS Coarse Aggregate quantity/m 3 obtained by ACI method is kg less than that obtained by IS Yield (i. e. density of concrete) is more in IS method of Mix Design. 2019, IRJET Impact Factor value: ISO 9001:2008 Certified Journal Page 2583
5 5. CONCLUSIONS As the strength requirement increases, the (w/c) Looking at the proportions, it can be said that the Mix design by IS code is in line with that by ACI From table 4 (ACI method), it can be depicted that (w/c) ratio to be used depends upon the required compressive strength. However, IS code gives the max. limits for free (w/c) ratios depending upon the exposure conditions for plain concrete & RCC work from durability point of view. Coarse Aggregates are more in IS method of mix design. Fine Aggregates are comparatively more in case of ACI More quantity of Fine Aggregates, obtained by ACI method, should presumably lead to more workability, owing to the fact that the fine aggregates act as ball bearings & provide lubricating effect to the mix. As the Fine Aggregates have the tendency of filling the voids, ACI method should give more strength due to enhanced particle packing. From table 5 (ACI method), it can be clearly seen that if the nominal maximum size of CA & fineness modulus of FA are not varied then volume of dry rodded CA per unit volume of concrete is same for any grade of concrete. In such a case, mass of the CA is a function of dry rodded density of CA. If CAs are well graded with all size factions, there will be less voids. This will lead to higher dry rodded density of CA. In ACI method, the mass of CA to be incorporated in concrete is independent of the (w/c) ratio. In IS method, as the (w/c) ratio decreases, the volume of CA increases. Vice versa is also true. Less the (w/c) ratio, more will be volume of CA which, in turn, leads to greater mass of CA. ratio lowers & CA content becomes comparatively more in IS At the same time, FA content becomes less. This sounds contradictory theoretically, because of the possibility that more the CA, more would be the voids, thereby decreasing the strength of the concrete. This paper was an attempt of comparing the two methods of Concrete Mix Design by randomly picking up a grade of M35. In doing so, certain modifications were done by manual judgment to fit to the requirements. The results obtained just show a general trend in connection with both the methods. The different assumptions & modifications, using experience & manual judgment, while carrying out Concrete Mix Design may lead to somewhat deviating results. One has to meticulously carry out Concrete Mix Design by both the methods & conduct a large number of trials in the laboratory for various grades of concrete in order to simultaneously satisfy strength & workability requirements. REFRENCES 1. Code of practice for plain and reinforced concrete (fourth edition), IS 456:2000, Bureau of India Standard, New Delhi. 2. Indian standard concrete mix proportioning  Guidelines (First revision) IS 10262:2009, Bureau of India Standard, New Delhi, India. 3. Standard practice for selecting proportions for normal, heavyweight, and mass concrete, ACI (1991), ACI Committee 211, Farmington Hills, MI, USA. 2019, IRJET Impact Factor value: ISO 9001:2008 Certified Journal Page 2584